Hindawi Advances in Civil Engineering Volume 2020, Article ID 1643529, 6 pages https://doi.org/10.1155/2020/1643529 Research Article Development of an Ensemble Intelligent Model for Assessing the Strength of Cemented Paste Backfill Yuantian Sun,1 Guichen Li ,1 Junfei Zhang,2 Junbo Sun,2 and Jiahui Xu1 1 School of Mines, Key Laboratory of Deep Coal Resource Mining, Ministry of Education of China, China University of Mining and Technology, Xuzhou 221116, China 2 Department of Civil, Environmental and Mining Engineering, The University of Western Australia, Perth 6009, Australia Correspondence should be addressed to Guichen Li; [email protected] and Qiusong Chen Received 13 March 2020; Accepted 13 March 2020; Published 16 April 2020 Academic Editor: Qiusong Chen Copyright © 2020 Yuantian Sun et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited. Cemented paste backﬁll (CPB) is an eco-friendly composite containing mine waste or tailings and has been widely used as construction materials in underground stopes. In the ﬁeld, the uniaxial compressive strength (UCS) of CPB is critical as it is closely related to the stability of stopes. Predicting the UCS of CPB using traditional mathematical models is far from being satisfactory due to the highly nonlinear relationships between the UCS and a large number of inﬂuencing variables. To solve this problem, this study uses a support vector machine (SVM) to predict the UCS of CPB. The hyperparameters of the SVM model are tuned using the beetle antennae search (BAS) algorithm; then, the model is called BSVM. The BSVM is then trained on a dataset collected from the experimental results. To explain the importance of each input variable on the UCS of CPB, the variable importance is obtained using a sensitivity study with the BSVM as the objective function. The results show that the proposed BSVM has high prediction accuracy on the test set with a high correlation coeﬃcient (0.97) and low root-mean-square error (0.27 MPa). The proposed model can guide the design of CPB during mining. 1. Introduction Cemented paste backﬁll (CPB) is widely used for mining operations in underground metal mines, in which tailings are normally used as main aggregates and they are mixed with cementitious material and water . CPB is normally ﬁlled into the underground stope, and thus, it plays a critical role in supporting the roof and surrounding rock mass after a certain period of dehydration and consolidation [2–5]. Compared with other backﬁll materials, CPB is an eco-friendly and economic mine composite due to the maximum utilization of mine waste, which attracts much attention these years [6–11]. Filling strength is the most important mechanical parameter that aﬀects ﬁlling quality, and unconﬁned compressive strength (UCS) is the most basic and key parameter to evaluate the ﬁlling strength of CPB . Generally, the UCS of CPB is obtained in the laboratory, similar to the strength evaluation of the concrete. However, when multiple parameters are related to UCS of CPB, experimental measurement is a tedious, time-consuming, and expensive method [13, 14]. Many scholars have put forward many methods to predict the strength of CPB such as empirical formula estimation, numerical simulation, and elastic mechanics analysis [15, 16]. It should be pointed out that the CPB is a multiphase composite and the mentioned methods normally cannot obtain accurate prediction results. To accurately predict the UCS of CPB, it is necessary to put forward simple and reliable methods. Recently, machine learning methods have been widely used for predicting the mechanical properties of construction materials [12, 17–23]. The assessment of the strength of CPB by artiﬁcial intelligence methods has also been presented. For instance, artiﬁcial neural network (ANN) considering inﬂuencing variables of CPB has been used to model the relationship between inputs and outputs [24, 25]. Furthermore, the evolutionary ANN method, namely, ANNbased methods, was proposed for estimating the UCS of CPB, by which the hyperparameters such as the number of 2 Advances in Civil Engineering (1) The support vector machine (SVM) and beetle antennae search (BAS) algorithms were combined to establish the evolutionary support vector machine model; (2) The strength properties of CPB was analyzed by conducting the experiments considering the key inﬂuencing variables, i.e., cement-coarse tailings ratio, solids-water ratio, ﬁne tailings percentage, and curing time (3) The UCS of CPB was directly estimated by considering the combined eﬀect of four key inﬂuencing variables (4) The sensitive analysis of the mentioned inﬂuencing variables of CBP was ﬁrst analyzed and discussed 2. Materials and Methods 2.1. Mechanical Tests. To prepare the CPB specimen, the grain size distribution of tailings and the mineralogical composition are necessary to determine. Thus, a laser diffraction analyzer was utilized for determining the size distribution of coarse tailings and ﬁne tailings. As we can see from Figure 1, there are two diﬀerent tailings of various sizes. To analyze the inﬂuence of ﬁne tailing on the strength of CPB is critical. The Portland cement P.O 32.5R was applied as a binder. The water obtained in this mine was used as the mixing water. According to the ﬁeld trial tests, coarse tailings-cement ratio (T/C) was set as 4, 6, 8, and 10, and the solids-water ratio (S/W) was set as 0.68, 0.70, and 0.72. The ﬁne tailings are as an admixture, and its percentage (FTP) was set as 0%, 10%, 15%, and 20%. The blinder and aggregates were mixed by using a mixer (UJZ-15) for 5 min. Then, the prepared mixture was poured into the molds (70.1 mm × 70.1 mm × 70.1 mm). The curing time in this study was set as 7, 28, and 60 days. The detailed statistics of variables of CPB are given in Table 1. A total of 435 specimens were completed, and they were used for obtaining the 100 Cumulative distribution (%) neurons and the structure of ANN are optimized by some global optimization algorithms, i.e., particle swarm optimization (PSO) and ﬁreﬂy algorithm (FA). Similarly, other normally used machine learning methods such as the random forest algorithm (RF) and RF-based models reported in the literature are also used for predicting the UCS of CPB . Although the above artiﬁcial intelligence methods (ANN, ANN-based, RF, and RF-based) were applied in strength prediction of CPB, they are limited in calculating eﬃciency and uncertain structures. Besides, there is no intelligent model for the prediction of UCS of CPB considering the overall eﬀect of cement-coarse tailings ratio, solids-water ratio, ﬁne tailings percentage, and curing time. Therefore, in this paper, the machine learning algorithms, support vector machine (SVM) that has the perfect ability in regression and classiﬁcation, and an excellent global optimization algorithm, beetle antennae search algorithm (BAS) that is used for selecting hyperparameters of SVM, were combined. Therefore, an evolutionary support vector machine model (BSVM) is proposed. Several contributions to the literature can be concluded as follows: 80 60 40 20 0 1 10 Particle size (mm) 100 1000 Fine tailings Coarse tailings Figure 1: Grain size distribution of coarse and ﬁne tailings. UCS values by conducting unconﬁned compressive tests according to ASTM C 39. 2.2. Model of Evolutionary Support Vector Machine (BSVM) 2.2.1. Support Vector Machine (SVM). SVM is normally applied for classifying the samples by the hyperplanes . When the hyperplane can make a large margin in two classes, the vectors corresponding to the hyperplanes are support vectors. The schematic diagram of the SVM is depicted in Figure 2. Generally, the hyperplane equation is as follows: f(x) � wT g(x) + b, (1) where w means an m-dimensional vector; b denotes the bias term; and when w and b are obtained, the x can be classiﬁed by the sign of f (x). For linear separable data, the following equation can be concluded as follows: yi wT g(x) + b − 1 ≥ 0. (2) The support vectors are on the hyperplane: yi wT g(x) + b � 1. (3) To minimize the ‖w‖2, the hyperplane can be found (‖w‖ is the Euclidean norm of w). 2.2.2. Beetle Antennae Search (BAS). BAS is a very famous metaheuristic algorithm, which is proposed recently . It can be used for global optimization problems. Nowadays, BAS has been widely utilized in obtaining hyperparameters in machine learning algorithms [20, 21]. In this algorithm, it simulated the beetles’ behavior, and the objective of its antennae is to ﬁnd the odor with high concentration. A typical ﬂow chart of BAS is shown in Figure 3. In this study, the hyperparameters of SVM (C, penalty coeﬃcient and c, kernel parameter) were tuned by BAS instead of trial-and-error methods. Advances in Civil Engineering 3 Table 1: Statistics of inﬂuencing variables. Variable Coarse tailings-cement ratio (T/C) Solids-water ratio (S/W) Fine tailings percentage (FTP) Curing time Min 4 0.68 0 7 Max 10 0.72 0.2 60 Mean 7 0.7 0.11 31.6 Standard deviation 2.2 0.02 0.07 21.8 Margin lane perp g hy atin r a p Se Support vector Figure 2: Diagram of SVM. Initalize the position of beetle Best solution Y N Fitness function of beetle Is current ﬁtness better than the best position Y N Update the best position Stopping criterion A step to left A step to right Unchange N Fitness of left antennae > Fitness of right antennae Y Set beetle direction and calculate ﬁtness of antennae Figure 3: Flow chart of BAS. 2.3. Performance Evaluation. According to the suggestion in previous studies, the training dataset and testing dataset are split into 70% dataset and 30% dataset, respectively. A 10-fold cross- validation method was applied. The correlation coeﬃcient (R) and root-mean-square error (RMSE) for evaluating the performance of the established model are deﬁned as follows: ∗ ∗ y − y N i i�1 yi − y �, ������������ R � ������������ 2 N N ∗ i�1 yi − y∗ i�1 yi − y2 ��������������� 1 N 2 RMSE � y ∗ − yi , N i�1 i (4) 4 Advances in Civil Engineering 0.3450 10 0.8000 10 0.9844 1.198 1.411 0 5 72 71 Solids-w 70 69 ater rati o (% 5 10 15 20 68 ) 1.624 1.468 1.801 2.135 2.469 0 5 1.837 2.050 72 UCS (MPa) 71 Solids-w 70 69 ater rati o (% 68 ) (a) 5 10 15 20 F per ine ta cen ilin tag gs e( %) Coarse tailings-cement ratio 1.134 0.7712 F p er i n e t a cen ilin tag gs e( %) Coarse tailings-cement ratio 0.5581 2.803 3.138 3.470 (b) 0.4900 10 1.268 1.656 2.045 2.434 0 5 72 71 Solids-w 70 69 ater rati o (% 5 10 15 20 ) 68 F per ine ta cen ilin tag gs e( %) Coarse tailings-cement ratio 0.8788 2.823 3.211 3.600 (c) Figure 4: UCS test results of CPB in 4D: (a) 7 days; (b) 28 days; (c) 60 days. where N means the numbers in the dataset; yi∗ and yi are the expected values and real values, respectively; and y and y∗ indicate the mean predicted values and mean actual values, respectively. 3. Results and Discussion 3.1. Results of UCS of CPB. Figure 4 shows the UCS of CPB combined with diﬀerent variables under diﬀerent curing times. It can be seen that the coarse tailings-cement ratio is the main index for determining the strength of CPB. With the increase of coarse tailings-cement ratio, the UCS of CPB increased obviously. Similarly, the UCS of CPB improved with the increase of the solids-water ratio. However, in terms of the eﬀect of ﬁne tailing percentage on CPB strength, it depends on the solids-water ratio. Speciﬁcally, when the solids-water ratio is between 68% and 70%, with the increase of the ﬁne tailing percentage, the UCS of CPB increased to the peak values and then declined. When the solids-water ratio is 72%, the UCS of CPB decreased slightly with the increase of ﬁne tailing percentage. The curing time played a positive eﬀect on the increase in the strength of CPB, which is consistent with the previous studies. 3.2. Results of Hyperparameter Tuning. In this study, BAS is applied to tune hyperparameters of SVM on the training set. RMSE is selected as the objective function. Figure 5 shows the RMSE versus iteration curve. It can be seen that RMSE decreases signiﬁcantly and is stable after 15 iterations, indicating that the BAS is eﬃcient in tuning hyperparameters. The ﬁnal hyperparameters of SVM are tabulated in Table 2. 3.3. Assessment of the Established Model. Figure 6 shows the correlation between predicted UCS values and actual UCS values on the training and test sets. A nearly linear relationship is observed with R values of 0.9701 and 0.973 on the training and test sets, respectively, indicating that the proposed SVM model can establish the relationship between the UCS of CPB and its inﬂuencing variables successfully. Besides, the low and similar RMSE values on the training (0.1798) and test (0.2674) sets suggest that no underﬁtting or overﬁtting phenomena are produced. 3.4. Analysis of the Variable Importance. The relative importance of the input variables is calculated using global sensitivity study, as shown in Figure 7. It can be observed Advances in Civil Engineering 5 0.3 T/C Inﬂucential variable 0.25 RMSE 0.2 0.15 4.4657 Time 3.1780 S/W 0.2304 FTP 0.0887 0.1 0 1 0.05 0 10 20 30 40 50 Iteration Figure 5: RMSE versus iterations. Table 2: The obtained hyperparameters of RF. Parameters C Γ Empirical scope [0.1, 1000] [0.001, 100] Initial 14 14 Results 65 1.01 3 Predicted UCS 2.5 5 Figure 7: Variable importance of CPB based on the BSVM. that the coarse tailings-cement ratio has the most signiﬁcant inﬂuence on the UCS of CPB with an inﬂuencing score of 4.46, followed by curing time (3.178) and solids-water ratio (0.23), while ﬁne tailings percentage is the least sensitive variable with an inﬂuence score of 0.088. This result agrees well with the previous study. It should be noted that the importance score is obtained by the dataset used in this paper. More accurate results can be obtained if more data samples are included in the dataset in the future. This study uses the BSVM for predicting the UCS of CPB. The hyperparameters of SVM are tuned by BAS. The BSVM can establish the relationship between the UCS of CPB and its inﬂuencing variables successfully, indicated by high correlation coeﬃcients on the training (0.97) and test (0.973) sets. Also, the calculated variable importance by sensitivity analysis shows the coarse tailings-cement ratio is the most important variable to UCS. In future work, the dataset will be enlarged by including more inﬂuencing variables and samples to improve the generalizability of the proposed model. Also, a graphical user interface will be implemented to facilitate the use of the model in designing CPB mixtures. 2 1.5 1 0.5 1 4 4. Conclusions RMSE = 0.1798 R = 0.9701 0.5 2 3 Importance score 1.5 2 Actual UCS 2.5 3 (a) 3.5 Predicted UCS 3 Data Availability RMSE = 0.2674 R = 0.973 The Microsoft Excel Worksheet data used to support the ﬁndings of this study are available from the corresponding author ([email protected]) upon request. 2.5 2 Conflicts of Interest 1.5 The authors declare that there are no conﬂicts of interest. 1 0.5 Acknowledgments 0.5 1 1.5 2 2.5 Actual UCS 3 3.5 (b) Figure 6: Comparison of UCS values. (a) Training dataset. (b) Testing dataset. This study was ﬁnancially supported by the “National Key Research and Development Program (grant number: 2016YFC0600901)” and “National Natural Science Foundation of China (grant numbers: 51574224 and 51704277)”. The authors are grateful to Huaibei Mining (Group) Co. Ltd. 6 The author thanks Dr. Zuqi Wang for her encouragement and help. References  C. Qi and A. Fourie, “Cemented paste backﬁll for mineral tailings management: review and future perspectives,” Minerals Engineering, vol. 144, p. 106025, 2019.  Y. Sun, G. Li, and J. Zhang, “Investigation on jet grouting support strategy for controlling time-dependent deformation in the roadway,” Energy Science & Engineering, vol. 8, no. 4, pp. 1–8, 2020.  Y. Sun, G. Li, J. Zhang, and D. Qian, “Experimental and numerical investigation on a novel support system for controlling roadway deformation in underground coal mines,” Energy Science & Engineering, vol. 8, no. 2, pp. 490–500, 2020.  Y. Sun, G. Li, J. Zhang, and D. Qian, “Stability control for the rheological roadway by a novel high-eﬃciency jet grouting technique in deep underground coal mines,” Sustainability, vol. 11, no. 22, p. 6494, 2019.  H. Basarir, Y. Sun, and G. Li, “Gateway stability analysis by global-local modeling approach,” International Journal of Rock Mechanics and Mining Sciences, vol. 113, pp. 31–40, 2019.  Y. Sun, G. Li, and J. Zhang, “Developing hybrid machine learning models for estimating the unconﬁned compressive strength of jet grouting composite: a comparative study,” Applied Sciences, vol. 10, no. 5, p. 1612, 2020.  Q. Chen, Q. Zhang, C. Qi, A. Fourie, and C. Xiao, “Recycling phosphogypsum and construction demolition waste for cemented paste backﬁll and its environmental impact,” Journal of Cleaner Production, vol. 186, pp. 418–429, 2018.  Q. Chen, Q. Zhang, A. Fourie, and C. Xin, “Utilization of phosphogypsum and phosphate tailings for cemented paste backﬁll,” Journal of Environmental Management, vol. 201, pp. 19–27, 2017.  Q.-S. Chen, Q.-L. Zhang, A. Fourie, X. Chen, and C.-C. Qi, “Experimental investigation on the strength characteristics of cement paste backﬁll in a similar stope model and its mechanism,” Construction and Building Materials, vol. 154, pp. 34–43, 2017.  C.-c. Qi, “Big data management in the mining industry,” International Journal of Minerals, Metallurgy and Materials, vol. 27, no. 2, pp. 131–139, 2020.  D. Wang, Q. Zhang, Q. Chen, C. Qi, Y. Feng, and C. Xiao, “Temperature variation characteristics in ﬂocculation settlement of tailings and its mechanism,” International Journal of Minerals, Metallurgy and Materials, 2020.  C. Qi, A. Fourie, Q. Chen, and Q. Zhang, “A strength prediction model using artiﬁcial intelligence for recycling waste tailings as cemented paste backﬁll,” Journal of Cleaner Production, vol. 183, pp. 566–578, 2018.  Z. Zhang, E. Wang, and N. Li, “Fractal characteristics of acoustic emission events based on single-link cluster method during uniaxial loading of rock,” Chaos, Solitons & Fractals, vol. 104, pp. 298–306, 2017.  Z. Zhang, E. Wang, Y. Zhang et al., “Analysis on the timefrequency characteristics of ultrasonic waveform of coal under uniaxial loading,” Fractals, vol. 27, no. 06, pp. 1950100– 1950123, 2019.  S. Xu, F. T. Suorineni, K. Li, and Y. Li, “Evaluation of the strength and ultrasonic properties of foam-cemented paste backﬁll,” International Journal of Mining, Reclamation and Environment, vol. 31, no. 8, pp. 544–557, 2017. Advances in Civil Engineering  W. Xu, X. Tian, and P. Cao, “Assessment of hydration process and mechanical properties of cemented paste backﬁll by electrical resistivity measurement,” Nondestructive Testing and Evaluation, vol. 33, no. 2, pp. 198–212, 2018.  J. Zhang, G. Ma, Y. Huang, J. sun, F. Aslani, and B. Nener, “Modelling uniaxial compressive strength of lightweight selfcompacting concrete using random forest regression,” Construction and Building Materials, vol. 210, pp. 713–719, 2019.  C. Qi, A. Fourie, and Q. Chen, “Neural network and particle swarm optimization for predicting the unconﬁned compressive strength of cemented paste backﬁll,” Construction and Building Materials, vol. 159, pp. 473–478, 2018.  J. Sun, J. Zhang, Y. Gu, Y. Huang, Y. Sun, and G. Ma, “Prediction of permeability and unconﬁned compressive strength of pervious concrete using evolved support vector regression,” Construction and Building Materials, vol. 207, pp. 440–449, 2019.  Y. Sun, J. Zhang, G. Li, Y. Wang, J. Sun, and C. Jiang, “Optimized neural network using beetle antennae search for predicting the unconﬁned compressive strength of jet grouting coalcretes,” International Journal for Numerical and Analytical Methods in Geomechanics, vol. 43, no. 4, pp. 801– 813, 2019.  Y. Sun, J. Zhang, G. Li et al., “Determination of Young’s modulus of jet grouted coalcretes using an intelligent model,” Engineering Geology, vol. 252, pp. 43–53, 2019.  J. Zhang, D. Li, and Y. Wang, “Toward intelligent construction: prediction of mechanical properties of manufactured-sand concrete using tree-based models,” Journal of Cleaner Production, vol. 258, Article ID 120665, 2020.  Y. Sun, G. Li, J. Zhang, and D. Qian, “Prediction of the strength of rubberized concrete by an evolved random forest model,” Advances in Civil Engineering, vol. 2019, Article ID 5198583, 7 pages, 2019.  L. Orejarena and M. Fall, “The use of artiﬁcial neural networks to predict the eﬀect of sulphate attack on the strength of cemented paste backﬁll,” Bulletin of Engineering Geology and the Environment, vol. 69, no. 4, pp. 659–670, 2010.  L. Orejarena and M. Fall, “Artiﬁcial neural network based modeling of the coupled eﬀect of sulphate and temperature on the strength of cemented paste backﬁll,” Canadian Journal of Civil Engineering, vol. 38, no. 1, pp. 100–109, 2011.  C. Qi, Q. Chen, A. Fourie, and Q. Zhang, “An intelligent modelling framework for mechanical properties of cemented paste backﬁll,” Minerals Engineering, vol. 123, pp. 16–27, 2018.